2. The component layer of a flexible pavement laid
over subgrade are
Granular base course
Bituminous binder course
Bituminous surface course
To serve as an effective drainage layer to drain
off the water entering into the pavement layers,
leading to the longitudinal road side drains such
that only a very small proportion of water
enters into the subgrade.
To serve as a structure component of the
flexible pavement structure by distributing the
wheel load stresses transmitted through the
surface course and base course.
4. The material used for GSB layer are
1. Crushed stone aggregates
3. Coarse sand and
4. Selected soil such as moorum with less fine and very
The specified requirements of material used for GSB layer
are as under
a)Passing 0.425 mm sieve shall have LL < 25% and PI < 6%
b)Fine passing 75u sieve, less than 10%
c)CBR value not less than 30%
-suggested by MORTH
5. The sub-base material is spread to uniform thickness
and specified cross slope using a motor grader by
adjusting the blade of grader.
The moisture content of the material is checked and
the additional quantity of the water required to bring
up to OMC is sprinkled.
6. The loose GSB layer is compacted by rolling, if the
compacted layer thickness is less than 100mm than
ordinary smooth wheel roller may be used; for
compacted thickness is more than 100mm than
compaction is done by vibratory roller of static weight
10 tonnes or more.
Rolling is done starting from lower edge and
proceeded toward the center, rolling speed is limited
to less than 5 kmph.
Rolling is continued till at least 98% of maximum
density of the material.
7. The IRC and MORTH have suggested the no of
tests to be conducted
Minimum of one moisture content test is to be
carried out per 250 m2 area and minimum of
density test per 500 m2 area on each compacted
The granular sub base course is considered as
the most important component of flexible
pavement layer which sustains the wheel load
stresses and disperses through larger area on
the GSB layer below.
The base course must have sufficient quality
and thickness to prevent failure in the subgrade
and/or sub base, withstand the stresses
produced in the base itself.
9. The common types of base course materials used in
India for the construction of flexible pavement are ‘wet
mix macadam’, ‘water bound macadam’, soil aggregate
mixes and stabilized soil mixes.
The flexible pavements of most of the important
highways are being constructed these days using
WMM as the base course.
‘Crusher run macadam’ also used for base course.
(Providing crushed stone aggregate, depositing on a
prepared surface by hauling vehicles, spreading and
mixing with a motor grader, watering and compacting
with a vibratory roller)
11. • Los Angeles abrasion value : less than 40%
Aggregate impact value : less than 30%
• Combined flakiness and elongation index : less than
• Plasticity index of material finer than 0.425 mm sieve :
less than 6
• MORTH have suggested that min of one set of
aggregate impact, flakiness index and elongation index
tests are to be conducted per 200 m3 of aggregate
and minimum of one density test per 500 m2 on each
12. Bituminous pavement layers form an important part of
the flexible pavement layer system. Different types of
bituminous layers are being used as surface course of
flexible pavement. Thin bituminous surface are
provided for low traffic load and thicker surface is
provided of heavier traffic load.
It is essential to provide an appropriate type of
interface treatment before laying any type of
bituminous layer over the another layer. If the
bituminous layer is to be laid over a sub-base layer, the
prime coat and tack coat are applied. If the bituminous
layer is to be laid over an existing bituminous surface
then only tack coat is applied.
13. Bituminous layer is consist of three different
1 Base course
2 Binder course
3 Surface course
14. Over GSB
The surface is thoroughly cleaned free of dust.
Prime coat is applied by spraying liquid
bituminous binder of low viscosity.
After curing of the prime coat , a tack coat is
applied by spraying liquid bituminous binder of
After that desired type of bituminous pavement
layer is constructed.
on construction of existing bituminous layer,
only tack coat is applied.
15. Spraying of liquid bituminous binder of a low viscosity
over a GSB is called application of prime coat or
priming. It is important part of preparation before
laying a bituminous pavement layer over a GSB.
Penetrate deep into the surface and seal the void on
Coat and bond the loose particles on the surface
Permit the tack coat to be applied over the prime
surface to provide proper adhesion between base and
bituminous pavement layer.
16. Tack coat is application of a small quantity of
liquid bituminous binder of low viscosity over
either a prime granular surface or existing
The main objective of tack coat is to provide
adequate interface bond between the receiving
pavement surface and the new bituminous
18. BM consist of crushed aggregate and
bituminous binder heated and mixed in a hot
mix plant at specified temperature, transported
to the site, laid with mechanical paver and
compacted by roller.
Two different gradation are used as suggested
20. The aggregate to be used for the BM layer shall
fulfil the specified gradation. Two type of
aggregate gradation have been specified by the
IRC which is as given below table
21. The base on which bituminous macadam is to be laid
shall be prepared, shaped and compacted to the
The prime coat and take coat are applied as specified.
The BM mix is prepared in a hot mix plant at specified
temperature, depending on the grade of the bitumen
The hot mix is transported to the construction site in
insulated covered truck.
The BM mix is spread using a mechanical paver.
Bituminous materials shall be laid and compacted in
layers, which enable the specified thickness, surface
level, regularity requirements and compaction to be
22. The initial or breakdown rolling shall be done with 8-
10 tonne static weight smooth-wheel rollers. The
intermediate rolling shall be done with 8-10 tonne
static weight or vibratory roller or with a pneumatic
tyre roller of 12 to 15 tonne weight, with a tyre
pressure of at least 0.56 Mpa. The finish rolling shall be
done with 6 to 8 tonne smooth wheel tandem rollers.
Rolling shall continue until the specified compaction is
The bituminous macadam shall be covered with either
the next pavement course or wearing course, as the
case may be, within a maximum of forty-eight hours.
23. This base course may be used
as base course of flexible
pavement in certain short road
or in small road project where
hot mix plant is not available.
The coarse aggregate of specified
size are first spread and compacted
well in dry state.
After compaction, hot bitumen
binder of specified grade is sprayed in large quantity.
24. BUSG consist of a two layer composite
construction of compacted crushed stone
aggregate with bituminous binder applied after
each layer and key aggregate placed on the top
surface of the second layer.
After first layer is compacted, the bitumen
binder is sprayed at specified rate which
penetrate into layer; then second layer is spayed
and compacted, binder sprayed, key aggregates
sprayed and compacted.
A thin bituminous surface course is laid over the base
course to prevent the entry of surface water into the
pavement layers during rains.
And also serve as a wearing course.
Types of thin bituminous surfacing
(i) Surface Dressing
(ii) 20 mm thick "open Graded Pre-mixed Bituminous
Carpet” with seal coat and
(iii) 20 mm thick "Mixed being Surface" or "Close
26. General features
Bituminous surface Dressing' (BSD) is provided over a
prepared base course or existing pavement to serve as
thin wearing coat.
The surface dressing does not add to the structural
stability or strength of the pavement nor will it
improve the existing riding quality of the pavement
surface. The DBS is a cost effective surface treatment
to provide a dust free and impermeable pavement
The IRC has provided specification for two types of
surface dressing work,
1 single coat surface dressing
2 two coat surface dressing
30. The receiving surface is prepared by patching the pot-
The surface is cleaned with a mechanical broom to
remove loose material and dust.
Bituminous binder of specified grade is heated to the
specified temp and is uniformly sprayed using a
mechanical sprayer at the specified rate.
Immediately after the application of the binder, the
selected aggregate for surface dressing is spread using
a mechanical grit spreader at specified rate.
Immediately after spreading the aggregates, the entire
surface is rolled using a pneumatic tyre roller or a 6 to
8 tonne smooth wheeled roller.
31. When paving bitumen is used as binder the
finished surface may be opened to traffic on the
32. In the case of two-coat surface dressing, after
first coat as given above is allowed for two to
three weeks before the application of the
The binder is applied at the same specified rate
and immediately the aggregate of next smaller
size is spread at the specified rate. Rolling is
done as before, soon after spreading the
33. Open graded premix carpet (Pc) consists of
coarse aggregates of nominal size 13.2 (passing
22.4 mm and retained on 11.2 mm) premixed
with a suitable type and grade of bituminous
binder, spread and compacted to a thickness of
20 mm followed by application of seal coat, to
serve as a thin surface course of the pavement.
34. Mixed seal surfacing (MSS) is a thin bituminous
surfacing and is also called ‘close graded premix
surfacing'. This consists of aggregates of specified
gradation premixed with a suitable grade of paying
grade bitumen binder in a hot mix plant, spread with a
mechanical paver and compacted to a thickness of 20
mm to form a thin surfacing.
As the premix is prepared using close graded
aggregates with adequate bitumen binder content, the
MSS forms non-porous surface course and
there is no need to apply seal coat as in the case of
open graded premix carpet.
35. This work shall consist of construction of
Bituminous Concrete, for use in wearing
courses. This work shall consist of construction
in a single layer of bituminous concrete on a
previously prepared bituminous bound surface.
Bitumen, Coarse Aggregates, fine aggregates,
Filter (shall consist of finely divided mineral
matter such as rock dust, hydrated lime or
36. The first course shall be laid upon a surface which is
dry, clean and free from standing water, and only
when weather conditions are suitable.
In the case of placing new asphaltic concrete
pavement, the base course shall have been previously
prepared with one uniform application of Prime Coat
prior to the delivery of the asphaltic concrete paving
In the case of asphaltic concrete overlay, the existing
pavement surface shall have been previously prepared
with one uniform application of Tack Coat.
The mixture shall be delivered to the job and placed at
a temperature optimum for proper compaction.
37. In no case shall the mixture be placed at a temperature
of less than 125°C nor greater than 155°C.
Pavers shall be equipped with hoppers and it will be
spread material evenly on the base course.
38. When laying the mixture, pavers shall operate
so as to provide as continuous an operation as
possible at a speed of between three meters
and six meters per minute.
Pavers shall be capable of spreading the
mixture, without segregation, in thicknesses of
not less than 25 mm and not more than 75 mm.
Placement widths shall vary from a minimum of
1.5 meters to a maximum of 4.5 meters.